Photocatalytic activity of Cr-doped TiO2 nanoparticles deposited on porous multicrystalline silicon films
© Hajjaji et al.; licensee Springer. 2014
Received: 28 April 2014
Accepted: 15 September 2014
Published: 2 October 2014
This work deals with the deposition of Cr-doped TiO2 thin films on porous silicon (PS) prepared from electrochemical anodization of multicrystalline (mc-Si) Si wafers. The effect of Cr doping on the properties of the TiO2-Cr/PS/Si samples has been investigated by means of X-ray diffraction (XRD), atomic force microcopy (AFM), photoluminescence, lifetime, and laser beam-induced current (LBIC) measurements. The photocatalytic activity is carried out on TiO2-Cr/PS/Si samples. It was found that the TiO2-Cr/PS/mc-Si type structure degrades an organic pollutant (amido black) under ultraviolet (UV) light. A noticeable degradation of the pollutant is obtained for a Cr doping of 2 at. %. This result is discussed in light of LBIC and photoluminescence measurements.
In the past two decades, we observed a revival and a rapid expansion in titanium dioxide (TiO2) research activities. It was shown that this semiconductor has a strong photocatalytic activity compared to other semiconducting oxides, owing to its chemical stability and to the easy control of doping as well as electrical conductivity. This led to extensive works aiming to achieve TiO2-based nanoscale structures having high photocatalytic activities. The present work aims to present a novel photocatalytic structure consisting of Cr-doped TiO2 thin films deposited on multicrystalline porous silicon (PS). PS has been widely explored for its strong visible room-temperature photoluminescence (PL) and for its high potential application in photovoltaics (PV)[1, 2]. TiO2 is often used in screen-printed solar cells[3, 4] as a standard antireflective (AR) coating. PS-coated TiO2 was found to reduce the trapping of surface charge carriers and to enhance the PS photoluminescence stability and the optoelectronic properties of PS-based Si solar cells. TiO2 films have been prepared by a variety of deposition techniques including chemical vapor deposition, sol-gel processing, reactive sputtering[8, 9], and pulsed laser deposition (PLD)[10, 11]. Previous investigations recognized TiO2 as a promising photocatalyst material for total destruction of common organic pollutants. However, the effective photoexcitation of TiO2 requires irradiation in the ultraviolet (UV) region due to its large bandgap (3.2 eV), which leads to a merely 5% of solar energy absorption. Considerable efforts have been devoted to improve TiO2 photocatalytic performance in the visible light range. Such efforts include nitrogen, phosphate, and transition metal ion doping, and surface modification with dyes or quantum dots. The photocatalytic activity of TiO2 (mainly the anatase phase) doped with metallic ions showed that charge recombination processes largely depend on both type and doping level of the metallic element. Small concentrations of transition metals (less than 1%) lead to a lot of traps for electrons and/or holes, which then increases the recombination processes. However, this low concentration is not sufficient to increase visible light absorption in TiO2. On the contrary, a high doping level of about 5% to 10% may lead to a beneficial shift of the absorption edge toward visible light via a narrowing of the TiO2 bandgap; however, new recombination centers simultaneously take place, which then increases the recombination rates. Therefore, it is important to solve the recombination problem by searching a compromise while moderately doping the TiO2 films. Cr doping was widely used to enhance light absorption of TiO2 in the visible light. However, it was observed that at a certain Cr doping level, an anatase-to-rutile structural transition occurs, leading to a degradation of the photocatalytic activity of the material. In this work, Cr-doped TiO2 films were prepared using the co-sputtering deposition technique. Our aim consists of enhancing the visible light absorption efficiency of the TiO2 films via Cr doping. The effect of doping content on the photocatalytic efficiency of TiO2 has been studied by using the amido black dye.
PS has a large absorption spectrum lying from UV to near infrared, while TiO2 has an absorption limited to an energy radiation as high as 3.2 eV (anatase phase). The adjunction of TiO2 to PS could in principle generate further excitons that may enhance the photocatalytic activity, by injecting electrons (holes) in the conduction (valence) band of TiO2, which in turn enhance the photodegradation via an increase of the carrier lifetime.
The experiments were carried out on p-type mc-Si wafer having a thickness of 330 μm and a resistivity of 0.5 to 2 Ω cm. PS is formed using the electrochemical anodization method, in an ethanoic hydrofluoric acid solution (HF (48 wt. %)/ethanol = 1:4). The current density and anodization time were set to 7 mA/cm2 and 15 min, respectively. Pure TiO2 and TiO2:Cr thin films were deposited by means of radio frequency (RF) magnetron co-sputtering (13.56 MHz) technique on the PS/mc-Si substrates. Technical details of the co-sputtering deposition conditions were reported elsewhere. The TiO2 target was submitted to an RF power of 360 W, while the Cr element target was sputtered with variable power values (Pcr) ranging from 8 to 150 W. The Cr content in the TiO2:Cr films increases with Pcr and can be adjusted, at will, from 2 to 17 at. % Cr. The TiO2:Cr films were deposited at approximately 550°C, with a thickness of about 120 nm. The crystallographic structure was examined by means of the X-ray diffraction (XRD) technique using a Philips X'pert MPD X-ray diffractometer (Cu Kα radiation, PANalytical B.V., Almelo, The Netherlands). The surface morphology of the treated PS surfaces was investigated by atomic force microcopy (AFM). The PL properties were analyzed using a cooled GaInAs detector and Ar+ ion laser excitation source (λ = 488 nm). The effect of PS and TiO2/PS on the minority carrier diffusion length (L) of the active mc-Si material was evaluated by means of light beam-induced current (LBIC) measurements using the 632-nm wavelength of a He-Ne laser. The effective minority carrier lifetimes (τeff) were measured by photoconductance technique (WCT-120). Finally, the photocatalytic activity of both undoped and Cr-doped TiO2 films was carried out on a special organic pollutant (amido black) using a multi-UV lamp photo-reactor having a UV output power of 1.4 W and a maximum spectral intensity at 352 nm. The photocatalytic activity was measured by measuring the concentration of amido black (AB) after 4 min of UV irradiation, using the 617-nm wavelength of a double beam UV-visible spectrophotometer.
Results and discussions
AFM images show that incorporation of chromium induces a textural modification of the film (Figure 2). In a previous work, X-ray photoelectron spectroscopy showed that the concentrations of CrO2 and Cr2O3 compounds increase with Cr content; it is obvious that for Cr concentration as high as 17 at. %, Cr exists in the TiO2 lattice as well in the form of CrO2 and Cr2O3 compounds. The level of oxidation state increases with decreasing size. We also demonstrated that at high Cr content and mainly after annealing, Cr doping leads to anatase-to-rutile transition as well as to the formation of a small nanoparticle size. We also believe that a composite electrode made of TiO2 (or Cr-doped TiO2)/Cr2O3 forms, as has been already demonstrated by XPS.
where x is the distance between the aluminum electrode and the laser beam, A is a constant mainly depending on the intensity of the laser beam and the penetration depth, and n is a constant depending on the surface recombination velocity. A decrease of the factor n would be related to the reduction of the surface recombination velocity as a consequence of the passivating effect.
Evolution of the effective diffusion length of the mc-Si wafer after PS and TiO 2 :Cr/PS treatments
[Cr] = 0 at. %
[Cr] = 2 at. %
[Cr] = 13 at. %
Evolution of the effective minority carrier lifetime of the mc-Si after treatment with PS and TiO 2 :Cr/PS
[Cr] = 0 at. %
[Cr] = 2 at. %
[Cr] = 13 at. %
One may notice (Table 2) that PS or TiO2:Cr/PS-treated mc-Si samples have higher effective minority carrier lifetime values as compared to the untreated mc-Si wafer. First, the formation of PS improves the effective minority carrier lifetime of the mc-Si wafer from 2 to 23 μs; this value reaches a maximum of 733 μs after depositing a 2 at. % Cr-doped TiO2 film. Beyond this Cr concentration, the effective minority carrier lifetime decreases. The notable enhancement of the effective minority carrier lifetime for a Cr doping of 2 at. % (Table 2) would be due to a double step passivation; the first one is PS-based (reduction of the surface recombination velocity), while the second one consists of a TiO2-based passivation of PS while choosing an adequate Cr doping. Figure 4 shows the PL spectra of TiO2:Cr/PS structures. We should keep in mind that the PL emission is exclusively coming from PS and that the most intense PL corresponds to a Cr concentration of 2 at. %; beyond this critical value, we notice a decrease of the PL intensity (Figure 4). Additionally, the PL band peak position is almost independent of Cr content. Usually, when PS is being oxidized, one may observe an enhancement of the PL intensity together with an energy shift of the PL band[23, 24]. Therefore, one may presume that the decrease of the PL intensity for Cr doping higher than 2 at. % (Figure 4) is due to the change of the PS surface passivation, probably due to the formation of chromium oxides (textural modification).
The decrease of the PL intensity (as Cr doping increases) could not be due to the anatase-to-rutile transition or to the doping itself, as only the PS surface is concerned; a surface textural (Figure 2) modification (due to an increase in Cr doping) could influence the PL intensity (increase of non-radiative charge carrier recombination in PS). On the other hand, the content of CrO2 and Cr2O3 forming during the co-sputtering of Ti and Cr together with the anatase-to-rutile transition depends essentially on Cr doping and experimental conditions.
Figure 5c shows the variation of rate constant K versus Cr concentration; K was calculated to be 0.0076 min-1 ± 2.165 10-4 for Cr (2 at. %)-doped TiO2. The photocatalytic activity of Cr(2 at. %)-doped TiO2 was found to be higher than that of the undoped TiO2 film; this can be related to the surface morphology and to the optical and optoelectronic properties of TiO2 doped with 2 at. % Cr. In fact, higher surface roughness (root-mean-square (RMS)) leads to an increase of the effective surface area and may then improve the photocatalytic activity; the RMS of the TiO2:Cr/PS structures increases from 17 to 43 nm as Cr doping varies from 0 to 4 at. %. Good photocatalytic response at an optimal concentration of 2 at. % Cr can also be explained by the increase in the minority carrier lifetime probably coming from carrier exchange with PS. This optimum could be explained by the fact that the presence of dopant prevents the recombination of exciton. Further increase in loading of Cr decreased the percentage of degradation of AB. This is due to the increased coverage of the semiconductor surface by the metal which decreases the surface adsorption sites expected to be available to the dye. The diminished penetration depth of light at higher Cr concentration could also prevent excitation of the semiconductor. In general, there are controversial results concerning the influence of Cr on the photocatalytic activity of the host material[26, 27]. It is then difficult to compare the reported results due to the variety of synthesis and experiment conditions, which in turn have substantial impacts on the material bandgap and performance photoactivity[26–30].
The observed optimum Cr concentration of 2 at. % could be related to an optimum incorporation of Cr3+ and Cr4+ ions in the TiO2 matrix and probably to the formation of Cr nanoparticles (existence of Cr-Cr bonds). The size of the nanoparticles can have a significant surface effect as the concentration of surface dangling bonds increases; the latter can serve as additional surface adsorption sites for the dye. On the other hand, oxidized small metallic nanoparticles are more active than reduced ones since the level of the oxidation state increases as the particle size decreases.
It is found that TiO2 sputtered on multicrystalline porous silicon substrates can effectively enhance the photocatalytic activity of this well-known photocatalyst. A noticeable improvement of the photocatalytic activity of Cr-doped TiO2 was obtained at a critical Cr doping of 2 at. %, which in turn improves the effective diffusion length and the effective minority carrier lifetime of the silicon substrate.
Further works are in progress to analyze the effect of Cr doping on the photocatalytic activity of TiO2, especially when the material is deposited with other techniques on substrates other than multicrystalline silicon, since the elaboration procedure and even the method of doping can affect the properties of the catalyst.
This work was financed by the Ministry of Higher Education, Scientific Research and Technology of Tunisia and Institut National de la Recherche Scientifique Canada, INRS-Énergie, Matériaux et Télécommunications (INRS-EMT).
- Zhang R, Chen Y, Zheng Y, Chen L: Research and progress of silicon luminescence. Chin J Lasers 2009, 36: 269–275. 10.3788/CJL20093602.0269View ArticleGoogle Scholar
- Yerokhov VY, Melnyk II: Porous silicon in solar cell structures: a review of achievements and modern directions of further use. Renew Sustainable Energy Rev 1999, 3: 291. 10.1016/S1364-0321(99)00005-2View ArticleGoogle Scholar
- Martinu L, Poitras D: Plasma deposition of optical films and coatings: a review. J Vac Sci Technol A 2000, 18: 2619–2645. 10.1116/1.1314395View ArticleGoogle Scholar
- Chatterjee S: Titania–germanium nanocomposite as a photovoltaic material. Sol Energy 2008, 82: 95–99. 10.1016/j.solener.2007.07.005View ArticleGoogle Scholar
- Kim KJ, Kim GS, Hong JS, Kang TS, Kim D: Characterization of a composite film prepared by deposition of TiO2 on porous Si. Sol Energy 1998, 64: 61–66. 10.1016/S0038-092X(98)00025-5View ArticleGoogle Scholar
- Hodroj A, Chaix-Pluchery O, Audier M, Gottlieb U, Deschanvres J-L: Thermal annealing of amorphous Ti–Si–O thin films. J Mater Res 2008, 23: 755–759. 10.1557/JMR.2008.0088View ArticleGoogle Scholar
- Zhang WF, Zhang MS, Yin Z: Microstructures and visible photoluminescence of TiO2 nanocrystals. Phys Status Solidi (a) 2000, 179: 319–327. 10.1002/1521-396X(200006)179:2<319::AID-PSSA319>3.0.CO;2-HView ArticleGoogle Scholar
- Dakka A, Lafait J, Abd-Lefdil M, Sella C: Optical study of titanium dioxide thin films prepared by R.F. sputtering. Moroccan J Condens Matter 1999, 1: 153–155.Google Scholar
- Laabidi A, Gaidi M, Guerin J, Bejaoui A, Maaref M, Aguir K: Alternating current investigation and modeling of the temperature and ozone effects on the grains and the grain boundary contributions to the WO3 sensor responses. Thin Solid Films 2009, 518: 355–361. 10.1016/j.tsf.2009.06.034View ArticleGoogle Scholar
- Ndione PF, Gaidi M, Durand C, Chaker M, Morandotti R, Rioux G: Structural and optical properties of epitaxial CaxBa1-xNb2O6 thin films grown on MgO by pulsed laser deposition. J Appl Phys 2008, 103: 033510. 10.1063/1.2838176View ArticleGoogle Scholar
- Amassian A, Gaidi M, Chaker M, Martinua L: Optical depth profiling of STO and electro-optic PLZT multilayer structures for active waveguide applications. J Vac Sci Technol 2006, 24: 55.View ArticleGoogle Scholar
- Bahnemann D: Photocatalytic water treatment: solar energy applications. Sol Energy 2004, 77: 445–459. 10.1016/j.solener.2004.03.031View ArticleGoogle Scholar
- Choi WY, Termin A, Hoffmann MR: The role of metal ion dopants in quantum-sized TiO2: correlation between photoreactivity and charge carrier recombination dynamics. J Phys Chem 1994, 84: 13669–13679.View ArticleGoogle Scholar
- Litter MI, Navío JA: Photocatalytic properties of iron-doped titania semiconductors. J Photochem Photobiol A Chem 1996, 98: 171–181. 10.1016/1010-6030(96)04343-2View ArticleGoogle Scholar
- Radecka M, Rekas M, Trenczek-Zajac A, Zarrzewska K: Importance of the band gap energy and flat band potential for application of modified TiO2 photoanodes in water photolysis. J Power Sources 2008, 181: 46–55. 10.1016/j.jpowsour.2007.10.082View ArticleGoogle Scholar
- Hajjaji A, Ben Rabha M, Janene N, Gaidi M, Bessais B, El Khakani MA: Minority carrier lifetime enhancement in multicrystalline silicon by means of a dual treatment based on porous silicon and sputter-deposition of TiO2:Cr passivation layers. Appl Surf Sci 2012, 258: 8046–8048. 10.1016/j.apsusc.2012.04.169View ArticleGoogle Scholar
- Davidson SM, Dimitriadis CA: Advances in the electrical assessment of semiconductors using the scanning electron microscope. J Microsc 1980, 118: 275–290. 10.1111/j.1365-2818.1980.tb00274.xView ArticleGoogle Scholar
- Ioannou DE, Gledhill RJ: SEM-EBIC and traveling light spot diffusion length measurements - normally irradiated charge-collecting diode. IEEE Trans Electron Devices 1983, 30: 577–580.View ArticleGoogle Scholar
- Khedher N, Hajji M, Bouaicha M, Boujmil MF, Ezzaouia H, Bessais B, Bennaceur R: Improvement of transport parameters in solar grade monocrystalline silicon by application of a sacrificial porous silicon layer. Solid State Commun 2002, 123: 7–10. 10.1016/S0038-1098(02)00206-5View ArticleGoogle Scholar
- Hajjaji A, Ben Rabha M, Janene N, Dimassi W, Gaidi M, Bessais B, El Khakani MA: Effect of dual treatment based on porous silicon and sputter-deposited TiO2 doped Cr film on the optoelectronic properties of monocrystalline Si. J Science JET CMarr 2012, 12: 1–4.Google Scholar
- Sproul AB: Dimensionless solution of the equation describing the effect of surface recombination on carrier decay in semiconductors. J Appl Phys 1994, 76: 2851. 10.1063/1.357521View ArticleGoogle Scholar
- Ben Rabha M, Bessaïs B: Enhancement of photovoltaic properties of multicrystalline silicon solar cells by combination of buried metallic contacts and thin porous silicon. Sol Energy 2010, 84: 486. 10.1016/j.solener.2010.01.007View ArticleGoogle Scholar
- Hajjaji A, Labidi A, Gaidi M, Ben Rabha M, Smirani R, Bejaoui A, Bessais B, El Khakani MA: Structural, optical and sensing properties of Cr-doped TiO2 thin films. J Sensors Letters 2011, 9: 1697–1703. 10.1166/sl.2011.1736View ArticleGoogle Scholar
- Hajjaji A, Ben Rabha M, Janene N, Gaidi M, Bessais B, El Khakani MA: Effect of dual treatment based on porous silicon and sputter-deposited TiO2 doped Cr film on the optoelectronic properties of monocrystalline Si. Appl Surf Sci 2012, 258: 8046. 10.1016/j.apsusc.2012.04.169View ArticleGoogle Scholar
- Wenhua L, Hong L, Saoan C, Jianqing Z, Chunan C: Kinetics of photocatalytic degradation of aniline in water over TiO2 supported on porous nickel. J Photochem Photobiol A 2000, 131: 125–132. 10.1016/S1010-6030(99)00232-4View ArticleGoogle Scholar
- Choi J, Park H, Hoffmann MR: Effects of single metal-ion doping on the visible-light photoreactivity of TiO2. J Phys Chem C 2010, 114: 783. 10.1021/jp908088xView ArticleGoogle Scholar
- Herrmann J-M: Detrimental cationic doping of titania in photocatalysis: why chromium Cr3+-doping is a catastrophe for photocatalysis, both under UV- and visible irradiations. New J Chem 2012, 36: 883–890. 10.1039/c2nj20914dView ArticleGoogle Scholar
- Trenczek-Zajac A, Radecka M, Jasinski M, Michalow K, Rekas M, Kusior E, Zakrewska K, Heel A, Graule T: Influence of Cr on structural and optical properties of TiO2:Cr nanopowders prepared by flame spray synthesis. J Power Sources 2009, 194: 104. 10.1016/j.jpowsour.2009.02.068View ArticleGoogle Scholar
- Michalowa KA, Otal EH, Burnata D, Fortunatoc G, Emerichd H, Ferri D, Heele A, Graule T: Flame-made visible light active TiO2:Cr photocatalysts: correlation between structural, optical and photocatalytic properties. Catal Today 2013, 209: 47–53.View ArticleGoogle Scholar
- Choudhury B, Choudhury A: Dopant induced changes in structural and optical properties of Cr3+ doped TiO2 nanoparticles. Mater Chem Phys 2012, 132: 1112–1118. 10.1016/j.matchemphys.2011.12.083View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.